Patent Publication Number: US-2022238868-A1

Title: Expanded hydrated vanadate

Description:
CROSS-REFERENCE TO RELATED APPLICATION 
     This application claims the benefit of U.S. Provisional Patent Application No. 62/848,458, filed on May 15, 2019, the disclosure of which is hereby expressly incorporated by reference in its entirety. 
    
    
     STATEMENT OF GOVERNMENT LICENSE RIGHTS 
     This invention was made with government support under Grant No. 1803256, awarded by the National Science Foundation. The government has certain rights in the invention. 
    
    
     BACKGROUND 
     Multivalent ions such as Mg 2+ , Zn 2+ , Ca 2+  and Al 3+  carry more charges per ion than Li +  or Na +  and are promising working ions in rechargeable batteries. Among all multivalent ions mentioned above, Zn 2+  has a smaller ionic radius of 0.74 Å in a six-fold coordination and Zn metal anode has a high volumetric capacity around 5850 mAh/cm −3 , thus aqueous zinc ion batteries (AZIBs) have generated interest. Before any new breakthrough happens in the present voltage-limited aqueous electrolytes, exploiting cathodes with high specific capacity is an effective way to achieve an increase in battery energy density. 
     Cathode materials for AZIBs mainly include manganese oxides, vanadium oxides, Prussian blue and its analogues, transition metal dichalcogenides and organic compounds. Manganese dioxides can be classified into one-, two- and three-dimensional tunnel structures that influence their electrochemical activities for Zn ion storage. The partially irreversible phase transition and the dissolution of active materials cause an unstable cycling performance. Prussian blue, the mixed-valence hexacyanoferrates with an open framework, has a tunable lattice spacing through introducing different transition metal cations, but the lower specific capacity of &lt;100 mAh/g can make them uncompetitive in comparison with manganese oxides of 300 mAh/g. Dichalcogenides deliver a considerable specific capacity around 200 mAh/g, however, the intrinsically low electrical conductivity and discharge voltage restrain their energy density and efficiency. Although organic compounds present a promising Zn ion storage capability, the dissolvable species formed in the cycling process cause a rapid capacity fading. 
     Cathode materials with improved specific capacity are essential to enabling more productive batteries, such as AZIBs. 
     SUMMARY 
     This summary is provided to introduce a selection of concepts in a simplified form that are further described below in the Detailed Description. This summary is not intended to identify key features of the claimed subject matter, nor is it intended to be used as an aid in determining the scope of the claimed subject matter. 
     In one aspect, a composition is provided comprising a cationically stabilized vanadate hydrate having a structure defined by layers of vanadium oxide separated by a cation and water, which provide spacing and stabilization between the layers. 
     In another aspect, an electrode is provided that includes a composition of cationically stabilized vanadate hydrates according to the embodiments described herein. 
     In yet another aspect, an aqueous battery is provided that includes a cathode that is an electrode as disclosed herein that includes a composition of cationically stabilized vanadate hydrates as disclosed herein. 
    
    
     
       DESCRIPTION OF THE DRAWINGS 
       The foregoing aspects and many of the attendant advantages of this invention will become more readily appreciated as the same become better understood by reference to the following detailed description, when taken in conjunction with the accompanying drawings, wherein: 
         FIG. 1A  is a graph illustrating the X-ray diffractometer (XRD) patterns of VOH and MnVOH in accordance with embodiments of the present technology. 
         FIG. 1B  is a graph of the FT-IR spectra with schematic functional groups of VOH and MnVOH in accordance with embodiments of the present technology. 
         FIG. 1C  is a graph of the Raman spectra with the function group models of VOH and MnVOH in accordance with embodiments of the present technology. 
         FIG. 1D  is a graph of the Raman details of the V—O group of VOH in accordance with embodiments of the present technology. 
         FIG. 1E  is a graph of the Raman details of Mn—O and V—O group from MnVOH in accordance with embodiments of the present technology. 
         FIG. 2A  is a TEM image with EDS mapping of MnVOH in accordance with embodiments of the present technology. 
         FIG. 2B  is a graph illustrating the differential scanning calorimetry curves of VOH and MnVO in accordance with embodiments of the present technology. 
         FIG. 2C  is a graph of the XPS spectrum of V2p 3/2  of MnVOH in accordance with embodiments of the present technology. 
         FIG. 2D  is a graph of the XPS spectrum of MnVOH collected from divalent Mn in accordance with embodiments of the present technology. 
         FIG. 3A  is a graph of current vs. voltage of MnVOH collected at a sweep rate of 0.1 mV/s in accordance with embodiments of the present technology. 
         FIG. 3B  is a graph comparing current vs. voltage curves of MnVOH and VOH in accordance with embodiments of the present technology. 
         FIG. 3C  is a graph of current vs. voltage of MnVOH collected at various sweep rates in accordance with embodiments of the present technology. 
         FIG. 3D  is a graph illustrating the relationship between peak currents and sweep rates for MnVO in accordance with embodiments of the present technology. 
         FIG. 4A  is a graph illustrating the voltage profiles of MnVOH at 50 mA/g in accordance with embodiments of the present technology. 
         FIG. 4B  is a graph illustrating the rate capability of MnVOH and VOH in accordance with embodiments of the present technology. 
         FIG. 4C  is a graph illustrating the cycling stability of MnVOH and VOH as cathodes in the aqueous Zn-ion battery in accordance with embodiments of the present technology. 
         FIG. 4D  is a graph illustrating the voltage profiles of MnVOH and VOH at the 1 st  and 50 th  cycles collected at 4 A/g in accordance with embodiments of the present technology. 
         FIG. 4E  is a graph illustrating the voltage hysteresis of MnVOH and VOH collected at 4 A/g in the 50 th  cycle in accordance with embodiments of the present technology. 
         FIG. 4F  is a graph illustrating the open circuit voltage degradations of MnVOH and VOH in batteries on the shelf in accordance with embodiments of the present technology. 
         FIG. 5A  is a graph illustrating the ex-situ XRD patterns of MnVOH at fully discharged and charged states in accordance with embodiments of the present technology. 
         FIG. 5B  is a graph illustrating the XPS spectra of V2p 3/2  at the fully discharged state in accordance with embodiments of the present technology. 
         FIG. 5C  is a graph illustrating the XPS spectra of V2p 3/2  at the fully charged state in accordance with embodiments of the present technology. 
         FIG. 5D  is a graph illustrating the evolution of Zn 2p3/2 spectra in accordance with embodiments of the present technology. 
         FIG. 5E  is a TEM image and EDS mapping of the fully discharged state in accordance with embodiments of the present technology. 
         FIG. 5F  is a TEM image and EDS mapping of the fully charged state in accordance with embodiments of the present technology. 
         FIG. 6A  is a GIIT plot of voltage versus time collected at a current density of 50 mAh/g for MnVOH and VOH in accordance with embodiments of the present technology. 
         FIG. 6B  is a graph of the reactive resistances during the charging and discharging process for MnVOH and VOH in accordance with embodiments of the present technology. 
         FIG. 6C  is a graph of the EIS spectra of VOH and MnVOH in accordance with embodiments of the present technology. 
         FIG. 6D  is a graph illustrating the relationship between real part of impedance and low frequencies for MnVOH and VOH in accordance with embodiments of the present technology. 
         FIG. 7A  is a graph of the XRD patters of NiVOH, CoVOH, and MnVOH in accordance with embodiments of the present technology. 
         FIG. 7B  is a graph of the rate capability of VOH, CoVOH, and NiVOH in accordance with embodiments of the present technology. 
         FIG. 7C  is a graph of the cycling stability of VOH, CoVOH, and NiVOH in accordance with embodiments of the present technology. 
         FIG. 8A  is a graph of the voltage discharge profiles of select transition metal stabilized VOH electrodes in aqueous Li-ion capacitors in accordance with embodiments of the present technology. 
         FIG. 8B  is a graph illustrating the voltage discharge profiles of select transition metal stabilized VOH electrodes in aqueous Li-ion capacitors in accordance with embodiments of the present technology. 
         FIG. 9A  is a graph illustrating the voltage profiles of transition metal stabilized VOH cathodes in Li-ion batteries in accordance with embodiments of the present technology. 
         FIG. 9B  is a graph illustrating the voltage profiles of transition metal stabilized VOH cathode in Na-ion batteries in accordance with embodiments of the present technology. 
         FIG. 10  is a graph illustrating the XRD patterns of Al (III), Mg (II), K (I) and Ca (II) stabilized VOH in accordance with embodiments of the present technology. 
         FIG. 11  is a graph illustrating the voltage profiles of an AlVOH cathode in an aqueous Zn-ion battery in accordance with embodiments of the present technology. 
         FIG. 12  is a graph illustrating the voltage profiles of a MgVOH cathode in an aqueous Mg-ion battery in accordance with embodiments of the present technology. 
         FIG. 13  is an SEM image of MnVOH in accordance with embodiments of the present technology. 
         FIG. 14  is a graph of XPS spectra of MnVOH and VOH in accordance with embodiments of the present technology. 
         FIG. 15  is a graph of XPS V2p spectrum of VOH in accordance with embodiments of the present technology. 
         FIG. 16  is a graph of the nitrogen-sorption isotherm of VOH and MnVOH in accordance with embodiments of the present technology. 
         FIG. 17  is a graph of the current vs. voltage curves of VOH in accordance with embodiments of the present technology. 
         FIG. 18  is a graph of the current vs. voltage curves of VOH collected at various rates in accordance with embodiments of the present technology. 
         FIG. 19  is a Ragone plot of the Zn-ion batteries with various cathodes in accordance with embodiments of the present technology. 
         FIG. 20  is a graph of the voltage profile of MnVOH and VOH at a current density of 4 A/g in accordance with embodiments of the present technology. 
         FIG. 21  is a graph of the XPS spectra Mn3s at fully charged and discharged states in accordance with embodiments of the present technology. 
         FIG. 22A  is an SEM image of a Zn anode in the pristine state in accordance with embodiments of the present technology. 
         FIG. 22B  is an SEM image of a Zn anode in the fully discharged state in accordance with embodiments of the present technology. 
         FIG. 22C  is an SEM image of a Zn anode in the fully charged state in accordance with embodiments of the present technology. 
         FIG. 23A  is an XRD pattern of CaVOH. 
         FIG. 23B  is a voltage profile of CaVOH at 0.5 A/g current density. 
         FIG. 24A  is an XRD pattern of KVOH. 
         FIG. 24B  is a voltage profile of KVOH across a range of current densities. 
         FIG. 25A  is an XRD pattern of AlVOH. 
         FIG. 25B  is a voltage profile of AlVOH at 50 mA/g current density. 
         FIG. 26A  is a diagram of a battery, in accordance with embodiments as disclosed herein. 
         FIG. 26B  is a diagram of a supercapacitor, in accordance with embodiments as disclosed herein. 
     
    
    
     DETAILED DESCRIPTION 
     The present disclosure generally relates to cation-stabilized expanded hydrated vanadates, electrodes made therefrom, and batteries incorporating cathodes made from the cation-stabilized expanded hydrated vanadate. Introducing cations, such as transition metal cations (TM), into the crystal lattice of hydrated vanadium pentoxide can stabilize its layered structure through cation-O bonds and provide several advantageous properties. 
     Aqueous zinc ion batteries have attracted extensive attention owing to their high safety, fast charge/discharge capability, long-term cycling stability, and low cost. The limits of cathodes restrain batteries&#39; energy density and efficiency. Exploring high-performance cathodes becomes an urgent and essential task and the requirements include high specific capacity, high discharge voltage, low self-discharge and highly reversible and stable cyclicity. Hydrated vanadium pentoxide (VOH) is a promising cathode for aqueous zinc ion batteries because of the high specific capacity as high as 400 mAh/g originating from the variable chemical states of vanadium cation. However, it suffers from the structural degradation that causes the cycling instability. The self-diffusion of zinc ions and electrons redistribution lead to a serious self-discharge and voltage degradation when the fully charged batteries are on the shelf. Currently, alkali and alkaline cation, such as Li + , Na + , K +  and Mg 2+ , are introduced into the interplanar of VOH to expand the lattice spacing to enhance the reaction kinetics and improve the rate capability and cycling stability. Conductive component like graphene is also used to obtain the composite for enhancing the electrical conductivity. These strategies, to some extent, alleviate the cycling degradation and provide fast channels for mass diffusion, but do not overcome the voltage degradation and self-discharge. 
     Layered materials offering sufficient intercalating channels and active sites for working cations transportation and accommodation have become the most competitive electrode materials for supporting commercial applications of the rechargeable batteries, especially the secondary Li ion batteries based on lithium cobalt oxide and graphite which have brought a revolution to portable electronics and communication. However, the layered cathodes in the flammable and highly volatile nonaqueous electrolytes introduce serious safety issues when oxygen released from the layered cathode penetrates to the anode causing thermal runaways. Aqueous electrolytes endow the rechargeable batteries improved safe protection, but the limited voltage window and single-electron carriers seriously restrain the energy density of batteries, even if high concentration salt solutions and “water-in-salt” electrolytes are introduced in Li-ion systems. 
     Layered vanadate compounds as one of the cathode categories for Zn-ion batteries can deliver a specific capacity as high as 400 mAh/g owing to the variable chemical valence of vanadium ion from 5+ to 3+ and its tunable interlayer distance for Zn-ion access and diffusion. Additionally, vanadium element has a considerable abundance of 190 ppm in the Earth&#39;s crust, leading to a lower cost than that of cobalt, which is widely used in commercial Li-ion batteries. Layered vanadium pentoxide, a common cathode for Li- and Na-ion batteries, in aqueous Zn ion batteries can deliver an increasing cycling gravimetric capacity due to the exfoliation of the initial chunks to allow more reactive sites. Hydrated vanadium pentoxide (V 2 O 5 .nH 2 O, VOH) has a bilayer structure and structural water molecules work as the pillar to expand the layer spacing to near 12 Å. Additionally, the shielding effect from water can decrease the interaction between cations and accelerate Zn ion diffusion. 
     In order to improve the reaction kinetics of VOH, some alien cations can be introduced into the interlayers to enlarge the spacing. It was found that the bigger radius of the alien cations could produce a larger layer distance and obtain a faster ion diffusion. For example, hydrated Mg 2+  with a radius of 4.3 Å creates an interlayer spacing of 13.4 Å in VOH, which is larger than 11.07 Å in hydrated Li +  expanded VOH because hydrated Li +  has a smaller radius of 3.8 Å. Similar studies have also been done with preinserted calcium and zinc cations. However, while the introduced cations play a role in expanding the lattice spacing to accelerate the ion diffusion, the electrochemical stability of host materials still suffers from structural degradation, especially with the possibility that alien cations deintercalate during the cycling processes because of the weak Van der Waals interaction between hydrated alien cations and oxygens from layered slabs of the host. 
     Thus, compared with the weak interactions, chemical bonding can lock the layered slabs and endow the host material a stable cycling stability for intercalation/deintercalation reactions without sacrificing the interplanar spacing. 
     Accordingly, the present technology provides cationically stabilized hydrated vanadate. For example, introducing divalent transition metal cations (TMs) into the crystal lattice of hydrated vanadium pentoxide can stabilize its layered structure through TM-O bonding. Compared with the weak Van der Waals&#39; force among water and alkali(ne) cation and terminal oxygen of [VO n ] polyhedral, the chemical bond of TM-O is stronger and endows a more stable crystal structure that accommodates the induced distortion and strain when zinc ions insert into or extract from the host lattice. 
     Cationically Stabilized Vanadate Hydrate Compositions 
     In one aspect, a composition is provided comprising a cationically stabilized vanadate hydrate having a structure defined by layers of vanadium oxide separated by a cation and water, which provide spacing and stabilization between the layers. 
     Hydrated vanadium pentoxide has a bi-layered structure that is constituted by two single layers of VO 5  pyramids. Water molecules reside into the interlayers, and the spacing distance of (001) plane without additional inserted material (molecules, ions, etc.) is 11.5 Å. This distance is adjustable from 8.7 to 13.8 Å through alien ions or organic molecules pre-insertion. In the disclosed embodiments alien cations are introduces of particular size and electronic characteristics are introduced into the interlayer along with water molecules. The cations both expand the interlayer spacing and also provide stabilization between the layers through bonding. 
     The materials can be made by methods know to those of skill in the art. As disclosed herein in the Examples, hydrothermal synthesis is a particularly effective synthetic approach to making many different species of cationically stabilized vanadate hydrates. 
     In certain embodiments, the cationically stabilized vanadate hydrate is present predominantly in a single phase. As used herein, the term “predominantly” indicates an amount of 95% or greater, by weight. In a further embodiment, the cationically stabilized vanadate hydrate is only present in a single phase. The purity of the single phase gives rise to the remarkable electronic properties as disclosed herein, particularly the large specific capacity when the materials are used as cathodes in electrochemical devices, such as batteries. 
     The phase of the resulting samples is always identified by X-ray diffractometer (XRD) and the collected pattern reflects the phase compositions. A single phase is indexed well with a corresponding standard pattern in the database. An amount of any second phase or impurity that exceeds 5 wt % is detectable by XRD and additional peaks will appear in the collected pattern. 
     In certain embodiments, the cationically stabilized vanadate hydrate has a greater interplanar spacing when compared to a vanadate hydrate formed by the same method but without the cation. 
     In certain embodiments, the cationically stabilized vanadate hydrate is structurally and thermally more stable when compared to a vanadate hydrate formed by the same method but without the cation. 
     In certain embodiments, the cationic stabilization results from an inclusion of a cation of optimal ionic radius selected from the group of manganese, chromium, titanium, scandium, iron, copper, nickel, cobalt, zinc, yttrium, zirconium, niobium, cadmium, aluminum, magnesium, potassium, calcium, sodium, and combinations thereof. As used herein, the term “optimal” ionic radius indicates an ionic radius that is large in relation to the interlayer distance. The cations disclosed herein have an ionic radius (in a 6-membered coordination) of 68 pm (for Al 3+ ) to 152 pm (for K + ). Therefore, in a further embodiment, the ionic radius of the cation is in the range of 68 pm to 152 pm. 
     In certain embodiments, the cationic stabilization results from an inclusion of a cation selected from the group of calcium, magnesium, potassium, aluminum, manganese, iron, cobalt, nickel, copper, zinc, and combinations thereof. Examples 1 and 2 describe the synthesis and characterization of cationically stabilized vanadate hydrates using these ions. 
     In certain embodiments, the composition has a chemical formula M x V 2 O 5 .nH 2 O, wherein M is a cation. In further embodiments, M is selected from the group of manganese, chromium, titanium, scandium, iron, copper, nickel, cobalt, zinc, yttrium, zirconium, niobium, cadmium, aluminum, magnesium, potassium, calcium, sodium, and combinations thereof. In further embodiments, M is selected from calcium, magnesium, potassium, aluminum, manganese, iron, cobalt, nickel, copper, zinc, and combinations thereof. 
     In further embodiments, the cation is bonded to the vanadium oxide. In yet further embodiments, the bonding is covalent, ionic, or Van der Waals. In a further embodiment the bonding is covalent. In a further embodiment the bonding is ionic. In a further embodiment the bonding is Van der Waals. 
     In certain embodiments, the composition consists essentially of the cationically stabilized vanadate hydrate. Small amounts of anions (e.g., from hydrothermal synthesis) may be incorporated into the composition. In a further embodiment, the composition consists of the cationically stabilized vanadate hydrate. 
     Electrodes Including Cationically Stabilized Vanadate Hydrates 
     In another aspect, an electrode is provided that includes a composition of cationically stabilized vanadate hydrates according to the embodiments described herein. 
     In certain embodiments, the electrode is configured for use in a battery.  FIG. 26A  is a diagram of a battery, in accordance with embodiments as disclosed herein. In  FIG. 26A , a Zn-ion battery includes a cathode as disclosed herein and the anode, as well as electrolyte. Zn-ions extract from the crystal lattice of the cathode and pass through the electrolyte to insert in or deposit on the anode in the discharging process. Upon charging, Zn-ions move in a reverse path. The insertion or extraction of ions cause a volume expansion or shrinkage of the crystal lattice. 
     In further embodiments, the battery is multivalent-ion battery. 
     In yet further embodiments, the battery is an aqueous zinc-ion battery (AZIB). In yet further embodiments, the batter is an Al-ion or Ca-ion battery. 
     In certain embodiments, the specific capacity is 250 mAh/g at 0.5 A/g or greater. In further embodiments, the specific capacity is 350 mAh/g at 0.5 A/g or greater. In further embodiments, the specific capacity is 400 mAh/g at 0.5 A/g or greater. 
     The charge transfer resistance and ion diffusion coefficient are also improved after the alien cation introduction, as illustrated in Example 1. 
     Supercapacitor Electrodes Incorporating Cationically Stabilized Vanadate Hydrates 
     Electrochemical capacitors, also known as supercapacitors, are of great interest for energy storage with numerous applications in back-up power sources, electric vehicles and intermittent wind and solar energy systems due to their high power density, long cycling time and great reversibility. Supercapacitors can be classified into electric double-layered capacitors (EDLCs) and pseudocapacitors (PCs) based on different charge storage mechanisms. The former is based on carbon materials which achieves energy storage by fast ion adsorption on the electrode surface, highly dependent on available surface area of materials, thus demonstrating high power density and long lifespan but low energy density. The latter always shows higher capacitance originating from pseudocapacitive materials (e.g. metal oxides, conductive polymers) triggering fast redox reactions at electrode/electrolyte interface, while exhibits limited cycling performance due to poor structural stability. Accordingly, the composites of carbon and redox-active materials always are fabricated to achieve maximization of electrochemical performance of capacitors combining the advantages of EDLCs and PCs simultaneously. 
     Vanadium pentoxide (V 2 O 5 ) is a promising electrochemically redox-active material with abundant resources, layered structure and high theoretical capacity (440 mAh g −1  as battery cathode), but the applications of which are limited by slow ion diffusion (10 −13 -10 −12  cm 2  s −1  for Li + ) and low electric conductivity (10 −3 -10 −2  S cm −1 ). Many efforts have been contributed to enhance electron transport in V 2 O 5 -based electrodes with the promise to achieve high-performance capacitors. Carbon materials are impressive supports for V 2 O 5  to partially relieve the constraint of conductivity and simultaneously to provide a large specific surface area with more active sites. For instance, reduced graphene oxide (rGO) and V 2 O 5  composites were fabricated to achieve high capacitance of 537 F g −1  at 1 A g −1  and 84% capacitance retention after 1,000 cycles compared to 30% of pure V 2 O 5  due to an enhanced conductivity. Carbon nanotubes (CNT) were introduced to V 2 O 5  nanowires systems to improve the energy density to 46.3 Wh kg −1  with the capacitance decay of 25% after 1,000 charge-discharge cycles. Nitrogen enriched mesoporous carbon spheres (n-MPC) were also excellent conductive templates for V 2 O 5 . The composites demonstrate 91 F g −1  of cell capacitance and 16% decay up to 2,000 cycles. However, the fast degradation of above carbon-V 2 O 5  electrodes still cannot satisfy the requirements for the long-life requirement for supercapacitors. 
     In certain embodiments, the electrode is configured for use in a supercapacitor.  FIG. 26B  is a diagram of a supercapacitor, in accordance with embodiments as disclosed herein. For supercapacitors, as illustrated in  FIG. 26B , cations and anions adsorb on the surface of the electrodes in the charging process and desorb reversibly in the discharging process. The volume change happens on the electrodes. 
     Expanded vanadate hydrates not only has the larger spacing distance but also the increased surface area. The surface of the resulting samples could adsorb ions as traditional supercapacitors do. In addition, the expanded interlayers allow the fast ion insertion and extraction to increase the pseudocapacitive contribution. The synergistic contribution could surmount the limitation of lower energy density in traditional supercapacitors. More importantly, the expanded interlayers present the probable possibility to the insertion of trivalent cation such as Al 3+ , benefiting to further increase the energy density of supercapacitors. 
     Batteries Incorporating Cationically Stabilized Vanadate Hydrates as an Electrode 
     In yet another aspect, an aqueous battery is provided that includes a cathode that is an electrode as disclosed herein that includes a composition of cationically stabilized vanadate hydrates as disclosed herein. 
     In certain embodiments, the aqueous battery is multivalent-ion battery. 
     In certain embodiments, the battery is an aqueous zinc-ion battery. 
     In certain embodiments, the cathode in the battery has a specific capacity is 250 mAh/g at 0.5 A/g or greater. 
     In certain embodiments, the cathode comprises manganese vanadate hydrate or potassium vanadate hydrate and the specific capacity is 400 mAh/g at 0.05 A/g or greater. 
     In certain embodiments, the battery has a capacity retention of 80% or greater. 
     In certain embodiments, the battery has a shelf life of 50 days or greater. 
     In certain embodiments, the battery has an energy efficiency of 70% or greater. 
     Methods of Synthesizing and Using the Cationically Stabilized Vanadate Hydrates 
     In additional aspects, methods of making the cationically stabilized vanadate hydrates are provided. In certain embodiments, the methods include hydrothermal synthesis of the cationically stabilized vanadate hydrates disclosed herein. Synthetic methods are described more fully in the Examples below. Each of the disclosed and claimed cationically stabilized vanadate hydrates disclosed herein can be made using the provided methods. 
     In further aspects, methods of using the cationically stabilized vanadate hydrates as electrodes in electrochemical energy storage devices are provided. In certain embodiments, the electrochemical energy storage devices is a battery or a supercapacitor. Such methods of use are described elsewhere herein and each of the disclosed and claimed cationically stabilized vanadate hydrates disclosed herein can be integrated as an electrode (e.g., a cathode) in an electrochemical energy storage device. Fabrication and performance of such devices are disclosed herein, particularly in the Examples. 
     The following Examples are included for the purpose of illustrating, not limiting, the disclosed embodiments. 
     Example 1. Preparation of Mn (II) Cation Expanded Hydrated Vanadium Pentoxide (MnVOH) 
     Mn (II) cation expanded hydrated vanadium pentoxide (MnVOH) is prepared through a hydrothermal method and shows much larger storage capacity and higher discharge voltage, and enhanced rate capability and cycling stability in comparison with VOH owing at least in part to enlarged interplanar spacing, stabilizing effect from Mn (II) pillars, catalytic effect from tetravalent vanadium cations, and improved charge and ion transport properties. The increased energy efficiency and reduced voltage degradation reveal a great potentiality for commercial applications. As one skilled in the art will appreciate from the disclosure herein, other transition metal cations (TMCs), such as Fe, Co, Ni, Cu, and Zn can also be introduced and present the same structures and functionalities to enhance the Zn-ion storage performance in an aqueous system, implying introducing TMCs is an effective and general strategy for improving the layered VOH cathode. Moreover, the transition metal cation expanded hydrated vanadate described herein can be used to enhance performance of Mg-ion, Na-ion, and Li-ion and Al-ion batteries and capacitors. 
     The description herein provides several specific embodiments of the present technology to better explain the present technology. However, as one skilled in the art will recognize from the disclosure herein, a variety of embodiments not specifically discussed herein are nevertheless included within the scope of the disclosure. For example, any of the embodiments and/or or methods discussed herein may utilize any suitable transition metal including, for example, manganese, chromium, titanium, scandium, iron, copper, nickel, cobalt, zinc, yttrium, zirconium, niobium and/or cadmium cations. In some embodiments, other ions, including, for example, aluminum, magnesium, potassium, calcium, and/or sodium, may be provided to stabilize VOH. Moreover, the stabilized hydrated vanadate may be applied in a number of contexts, including, for example, to improve zinc, lithium, magnesium, aluminum, and/or sodium ion batteries. 
     Methods of Preparing Select Embodiments of the Present Technology 
     All chemicals can be used as received without purification. 2 mmol of V 2 O 5  (e.g., 99.6+%, Sigma-Aldrich) can be dissolved into 50 mL of DI H 2 O with 2 mL of H 2 O 2  (e.g., 30%, Fisher chemical), and 1 mmol of MnSO 4 .10H 2 O (e.g., 98.3%, Fisher scientific) can be dissolved separately into 30 mL of DI water. Two solutions can be admixed and transferred to a 100 mL (internal diameter of 42 mm with a height of 72 mm) Teflon lined stainless steel autoclave and heated to and held at 120° C. for 6 h. Brick red precipitates can be collected by centrifugation and washed by water and ethanol for three times. The collected precipitates can be dried at 70° C. overnight in an electric oven and turned greenish. The resulting product (MnVOH) can be further dried at 120° C. in a vacuum oven. VOH can be synthesized with the same procedure and processing conditions without Mn (II) sources, 80 mL of DI water can be used in order to attain the same internal reactive pressure in the Teflon bottle and the resulting product can be dried by a freezing dryer at −52° C. For Fe (II), Co (II), Ni (II), Cu (II), Zn (II), Ca (II), Mg (II), Al (III) and K (I) stabilized samples, their sulfate salts can be used to synthesize the desired samples and the processes can be identical to the MnVOH synthesis. 
     Phase identification can be carried out by a Bruker X-ray diffractometer (e.g., D8 Discover with IμS 2-D detection system) at an accelerating voltage of 50 kV and a working current of 1000 μA. A Fourier Transform Infrared Spectrometer (e.g., FT-IR, Bruker, VERTEX 70) can be used to collect the functional groups&#39; stretching or bending information from 400 to 4500 cm −1  and a Renishaw InVia Raman Microscope equipped with the Leica DMIRBE inverted optical microscope, for example, can also be used to obtain the chemical bond information by one of the laser excitation sources at 514 nm. A differential scanning calorimeter (e.g., DSC 3+ STAR e  System, Mettler Toledo) can be adopted to analyze the thermal stability of sample within 40-700° C. in a flowing nitrogen gas (50 sccm). The microstructures of samples can be observed by a scanning electron microscope (e.g., SEM, FEI Sirion) at a working voltage of 5 kV and a scanning transmission electron microscope (S/TEM, Tecnai G2 F20) with an accelerating voltage of 200 kV. The surface chemical states of samples can be determined, for example, using a Kratos Axis Ultra DLD X-ray Photoelectron Spectroscopy system (XPS) with an AlKα radiation source that can be operated at 10 mA and 15 kV, and with a charge neutralizer. The angle between the specimen normal and the spectrometer can be 0°. 
     For the electrode preparation, the active material can be mixed with conductive carbon and polyvinylidene fluoride (PVDF) binder in a weight ratio of 7:2:1 in N-Methyl-2-Pyrrolidone (NMP) solvent to obtain a slurry that can be pasted on a current collector—titanium foil. The prepared electrodes can be dried in a vacuum oven at 120° C. overnight. The mass loading of active materials is about 3-4 mg/cm 2 . Zn metal can be used as the anode and 80 μL of 3 M zinc trifluoromethanesulfonate (98%, Zn(CF 3 SO 3 ) 2 ) aqueous solution can be injected into the batteries as the electrolyte. A glass fiber filter (e.g., Whatman, Grade GF/A) can be used as the separator. The redox characteristics of cathodes can be tested by cyclic voltammogram (CV) on a Solartron electrochemical station (SI 1287) equipped with an electrochemical impedance spectroscopy system (e.g., EIS, SI 1260). Galvanostatic intermittent titration technique (GITT) can be applied to analyze the reaction and diffusion kinetics at a current density of 50 mA/g and the charging/discharging time and interval of 10 min for each step. The Galvanostatic charge and discharge tests can be conducted, for example, by a Neware tester (CT-4008). The working voltage of cells can be set from 0.2 to 1.6 V versus Zn 2+ /Zn, and the EIS measurements have a frequency range between 10 5  and 0.01 Hz. As one skilled in the art will appreciate, the values and steps described herein may be altered while remaining within the scope of the present technology. 
     Select Embodiments of the Present Technology 
       FIG. 1A  compares the XRD patterns of MnVOH and VOH, in which VOH is well indexed with the standard peaks (V 2 O 5 .nH 2 O, PDF 40-1296) and MnVOH shows the same diffraction peaks as reported M x V 2 O 5 A y .nH 2 O (M=cations, A=anions). However, the Miller indices corresponding to crystallographic planes does not exist in the current database. The structure of M x V 2 O 5 A y .nH 2 O may include stacked V—O double layers and the adjacent layers can be separated by water and cations and anions added in the preparation. The strongest peak at 6.8° in MnVOH corresponds to a larger lattice spacing of 12.9 Å and VOH has the strongest peak at 7.4° with a lattice spacing of 11.9 Å that agrees with the reported ˜11.5 Å, suggesting the introduction of Mn (II) with water together can expand the interlayer spacing further as found in Mg preinserted VOH. In the FTIR spectra ( FIG. 1B ), peaks at 461 and 737 cm −1  originates from the symmetric stretching vibration of the O—V—O bonds and the peak located at 992 cm −1  can be attributed to the stretching vibration of the V═O bonds. The bending and stretching vibration of O—H from structural water appears around 1612 and 3450 cm −1 , respectively. Upon careful examination, a slight redshift (2-5 cm −1 ) of V—O vibrations appears in MnVOH in comparison with VOH, suggesting the V—O bond becomes weak because a fraction of V 5+  is reduced to V 4+  in MnVOH, the details on chemical states will be discussed further with the XPS results. The similarity in FT-IR spectra reveals similar crystal structures in both samples. Raman spectra ( FIG. 1C ), as the complementary fingerprints of samples to the FT-IR spectra, were collected. The peak located at 159 cm −1  comes from the bending vibration of the —O—V—O—V— chains, which implies an a-directional compressive deformation in the lattice. A blue shift of 4 cm −1  in MnVOH verifies the stronger compression along the a-direction due to the possible electrostatic interaction between Mn (II) and O. The bending vibration of the V═O bond formed by terminal O and center V cation appears at 264 cm −1 , and the red shift of 4 cm −1  in MnVOH means the elongation of V═O along the c-direction, consistent with the XRD results of the lowest angle. The board peak around 352 cm −1  is related to the librational motions of water. The triply coordinated O 3  by three V cations forms a V 3 —O bond that connects three edge sharing VO 5  pyramids in the crystal structure and is reflected by a stretching signal at 512 cm −1  and a red shift of 5 cm −1  in MnVOH suggests a lattice expansion along the b-direction. The bridging O links two corner-sharing VO 5  polyhedra and stretching vibration of V 2 —O appears at 706 cm −1 , and the peak at 674 cm −1  from stretching of V 2 —O suggests a partially disordered V—O—V connection existed in the host lattice. The weakened peak at 674 cm −1  in MnVO reveal a better crystallinity and the possible reason is that the introduced Mn (II) makes the arrangement of V and O to be more orderly because the interaction among the three ionic species. The peak at 891 cm −1  is attributed to the stretching of V—OH 2 . A weakened V—OH 2  bond appears in MnVOH because of the red shift, which implies water may have more rotational freedom in the interlayer. The competing interaction from Mn (II) and water could influence the bond strength of V—OH 2 . Compared the spectra of 600-800 cm′ of both samples, a broad peak appears at 674 cm −1  in MnVO rather than the sharp peak in VOH. Lorentz functions were used to obtain the details of chemical bonds, two discernable peaks at 674 and 706 cm −1  fit well with the stretching of V 2 —O in VOH ( FIG. 1D ), and a weak peak at 652 cm −1  corresponds to the vibration of Mn—O bond in MnO 6  octahedral of MnVOH ( FIG. 1E ), suggesting Mn (II) ions connect [VO n ] layers by chemical bonds. It should be mentioned that the bending or stretching signal of sulfate anion is not detected in Raman or FT-IR spectra, demonstrating no sulfate anion in MnVOH. Based on the structural comparison, MnVOH can have at least two possible structures. One is the bi-layer structure in which Mn (II) cations reside into the interlayers like a slight structure distortion in VOH, it can be called by a pre-inserted cation as sodium in V 2 O 5 . The other is to form a new phase as MnV 12 O 31 .10H 2 O (PDF 47-0146) which has the same XRD pattern as M x V 2 O 5 A y .nH 2 O. For the former, preinserted cations, such as Li +  and Mg + , in VOH seldom cause a big difference in the XRD patterns. The changes in the XRD pattern means the formation of new phases, but the analysis based on the FT-IR and Raman spectra demonstrate both samples have similar chemical bonds. Combining the structural information discussed above, MnVOH is likely to have a similar crystal structure as VOH and the preinserted Mn (II) in the interlayer forms the chemical bonds. 
       FIG. 2A  shows TEM images in which MnVOH comprises nanosheets. The nanosheets aggregate to form a micro-flower-like shape as observed by SEM ( FIG. 13 ). EDS mapping collected by TEM exhibits homogeneous element distributions of Mn, V and O in the resulting MnVOH sample, and the lattice spacing of 12.9 Å is in accordance with the XRD results. No sulfur was detected, which supports the argument about no anion (SO 4   2− ) in MnVOH interlayers as mentioned in the structural analysis. To confirm the effects of Mn (II) on the structural stability, DSC/TGA can be used to analyze the water loss and possible phase transition in the heating process. Water loss in both samples ( FIG. 2B ) accompanied with a continuous endothermal process is reflected by two weak peaks at 150 and 380° C. and the endothermal peak appearing around 685° C. is attributed to the melting of V 2 O 5 . It is worth noting that the end temperature for water loss from MnVOH (475° C.) is higher than that from VOH (380° C.) as marked by the dotted lines, suggesting water has a better structural stability derived from the interaction by Mn in MnVOH. The water content in MnVOH (15 wt %) is less than that in VOH (17 wt %). The introduction of Mn (II) could induce a change in chemical valence of V 5+  because of the electroneutrality required in the lattice. Survey XPS spectra ( FIG. 14 ) compare the characteristic peaks and Mn2p signal is only detected in MnVOH, which agrees with the elements in the XRD detected phase. No signal relating to S is detected in either samples, demonstrating no sulfate anion in MnVOH and supporting that the above-recited structure is reasonable. Characteristic peaks at 517.4 and 517.0 eV in the XPS spectrum of V2p 3/2  ( FIG. 2C ) are originated from V 5+ , the difference of binding energy means the local chemical surroundings are different for some V 5+ , in particular Mn (II) at 642.2 eV ( FIG. 2D ) and V 4+  at 516.4 eV. The detected divalent state of Mn cation verifies no oxidizing reaction happens on Mn (II) in the synthesis processes. The ratio of V 4+  in MnVOH and VOH are 18.9% and 13.2% ( FIG. 15  and  FIG. 2C ), respectively, determined by evaluating the integrated area in the fitting spectra. The appearance of V 4+  in VOH is possibly from a reduction reaction between V 2 O 5  and H 2 O 2  to form VO(O 2 ) +  in the synthesis process. More V 4+  detected in MnVOH is attributed to the introduced Mn (II) and the appearance of V 4+  implies oxygen vacancies in VOH and MnVOH as reported in V 2 O 5  or VOH. The impacts from oxygen vacancies are close in both samples because the similar amounts of V 4+ , thus the differences on electrochemical performances derives from the introduced Mn (II). V 4+  has a bigger ionic radius of 72 pm than that of 68 pm for V 5+  in a six coordination, which further expands the lattice spacing. At the same time, V 4+  possesses one electron in the 3d orbital beneficial for enhancing the electrical conductivity and catalyzing the electrochemical reaction; when oxygen vacancies are introduced, the number of d orbitals located at the bottom of the conduction band and the upper of the valence band increases. Both samples have a similar surface area of 50 m 2 /g ( FIG. 16 ), and it is unlikely that their surface area would make significantly different influences on the electrochemical performances. 
     Redox reaction in MnVOH was analyzed by the CV test and two pairs of peaks are shown in  FIG. 3A , the peak pair resided at higher voltage (1 V) is related to redox pair of V 5+ /V 4+  and the transition of V 4+ /V 3+  pair appears around 0.5 V. The overlapped CV curves in the first three cycles reflect a reversible reaction of MnVOH cathode in the aqueous Zn-ion battery. An interesting phenomenon is that the first discharge peak around 1 V shifts to a higher voltage in the subsequent cycles, possibly attributed to the local chemical surroundings change after Zn ion insertion. However, VOH has deviating peaks in the first three cycles and the discharge peaks shifts to lower voltage upon cycling ( FIG. 17 .)  FIG. 3B  compares the CV curves of both cathodes collected at 0.1 mV/s and smaller voltage differentiations in redox pairs of MnVOH as listed in Table 1, meaning MnVOH cathode has a smaller polarization and better reactive kinetics in the electrochemical processes. To analyze the reaction kinetics, various sweeping rates of CV curves were collected as shown in  FIG. 3C  and cathodic peaks shift toward higher voltages and anodic peaks move back to lower voltages with the increasing sweeping rates owing to the polarizations, especially phase transition happening in the electrode. Peak currents (i) and sweep rates (v) obey a power-law relationship that is described by 
         i=av   b ,  (1)
 
     where a and b are variables. b value of 1 indicates surface capacitance dominated charge storage and 0.5 is indicative of a mass diffusion-controlled charge storage. The b values of peaks a-d in MnVOH are 0.65, 0.86, 0.81 and 0.84 ( FIG. 3D ), whereas the values of peaks a′-d′ from VOH are 0.65, 0.76, 0.81 and 0.73 ( FIG. 18 ). These suggest both samples have the considerable kinetics and the electrochemical reactions are limited by ion diffusion and capacitor-like behavior partially contributes to the charge storage. 
     
       
         
           
               
             
               
                 TABLE 1 
               
             
            
               
                   
               
               
                 The redox pairs and voltage differentiation in both cathode materials 
               
            
           
           
               
               
               
            
               
                 Samples ID 
                 Redox pairs (V) 
                 Differentiation (V) 
               
               
                   
               
               
                 VOH 
                 1.15/0.93 
                 0.23 
               
               
                   
                 0.69/0.48 
                 0.21 
               
               
                 MnVOH 
                 1.01/0.98 
                 0.03 
               
               
                   
                 0.61/0.52 
                 0.09 
               
               
                   
               
            
           
         
       
     
     Voltage profiles of MnVOH is shown in  FIG. 4A  and the delivered specific capacity is 415 mAh/g at a current density of 50 mA/g, which is higher than that of other vanadium-based cathodes, such as Li intercalated V 2 O 5 .nH 2 O, Na 2 V 6 O 16 .3H 2 O, H 2 V 3 O 8 , VO 2 , LiV 3 O 8 , or Mg x V 2 O 5 .nH 2 O. The sloping curves agree with the board redox peaks in CV test, and the increased voltage and overlapped curves in the subsequent cycles suggests the highly reactive reversibility. In the rate capability tests ( FIG. 4B ), MnVOH electrode with a mass loading of 3-4 mg/cm 2  delivers an initial specific capacity of 380 mAh/g at a current density of 0.5 A/g, and VOH has a capacity of 287 mAh/g. The difference is that VOH presents a capacity increase to 326 mAh/g after the first five cycles, but MnVOH displays a relatively stable capacity at 371 mAh/g. With current density increasing from 1, 2, 4 to 8 A/g, MnVOH delivers the specific capacities of 347, 310, 268 and 214 mAh/g, respectively, and VOH exhibits the capacities of 280, 237, 179 and 124 mAh/g at the corresponding conditions. The capacity retention in MnVOH is 56% that is higher than that of 38% in VOH at 8 A/g compared with their capacities at 0.5 A/g, it is also more superior in comparison with VO 2  and Mg x V 2 O 5 .nH 2 O (Table 2). 
     
       
         
           
               
             
               
                 TABLE 2 
               
             
            
               
                   
               
               
                 Comparison of the cathodes for Zn-ion batteries 
               
            
           
           
               
               
               
               
            
               
                   
                 Voltage 
                 Specific capacity/ 
                 Cycling 
               
               
                 Cathode 
                 window 
                 Rate performance 
                 performance 
               
               
                   
               
               
                 MnO 2   
                 1.0-1.8 V 
                 285 mAh/g at 103 mA/g 
                 92% over 5,000 cycles at 
               
               
                   
                   
                   
                 1.5 A/g 
               
               
                 V 2 O 5   
                 0.4-1.4 V 
                 224 mAh g −1  at 100 mA/g 
                 121 mAh g −1  maintained 
               
               
                   
                   
                   
                 over 400 cycles at 1 A/g 
               
               
                 Na 0.33 V 2 O 5   
                 0.2-1.6 V 
                 367 mAh/g at 100 mA/g 
                 93% capacity retention 
               
               
                   
                   
                   
                 over 1,000 cycles at 1 A/g 
               
               
                 Na 2 V 6 O 16   
                 0.2-1.6 V 
                 352 mAh/g at 50 mA/g 
                 90% capacity retention 
               
               
                 1.63H 2 O 
                   
                   
                 over 6,000 cycles at 5 A/g 
               
               
                 Zn 0.25 V 2 O 5   
                 0.5-1.4 V 
                 282 mAh/g at 200 mA/g 
                 81% capacity retention 
               
               
                   
                   
                   
                 after 1,000 cycles at 2.4 A/g 
               
               
                 VO 2 (B) 
                 0.3-1.5 V 
                 357 mAh/g at 100 mA/g 
                 91.2% capacity retention 
               
               
                   
                   
                   
                 after 300 cycles at 0.1 A/g 
               
               
                 CuHCF 
                 0.2-1.2 V 
                 56 mAh/g at 20 mA/g 
                 77% capacity retention 
               
               
                   
                   
                   
                 after 20 cycles at 0.02 A/g 
               
               
                 ZnHCF 
                 0.8-2.0 V 
                 65 mAh/g at 60 mA/g 
                 76% capacity retention 
               
               
                   
                   
                   
                 after 100 cycles at 0.3 A/g 
               
               
                 Mg x V 2 O 5  · nH 2 O 
                 0.1-1.8 V 
                 353 mAh/g at 50 mA/g 
                 97% capacity retention 
               
               
                   
                   
                   
                 after 2,000 cycles at 5 A/g 
               
               
                 MnVOH 
                 0.2-1.6 V 
                 415 mAh/g at 50 mA/g 
                 96% capacity retention 
               
               
                   
                   
                   
                 after 2,000 cycles at 4 A/g 
               
               
                   
               
            
           
         
       
     
     When the current densities decrease back to 0.5 A/g from 8 A/g, the capacities recover to the initial values, suggesting a stable crystal structure and great electrochemical reversibility. During the high current cycling tests ( FIG. 4C ), MnVOH presents excellent stability after a slight capacity increase owing to the electrolyte penetration and electrochemical activation in the first several cycles. The stable specific capacity is around 260 mAh/g that closes to the result from rate test at the same current density of 4 A/g. However, the specific capacity of VOH decreases rapidly and capacity retention is 66% over 500 cycles, which is lower than 96% capacity retention over 2,000 cycles in MnVOH. The capacity retention of MnVOH is also higher than that of Zn 0.25 V 2 O 5 .nH 2 O (80% over 1,000 at 2.4 A/g) and LiV 2 (PO 4 ) 3  cathode (˜75% over 4,000 cycles at 1.5 A/g). The maximum energy and power densities of MnVOH are 267 Wh/kg and 5,791 W/kg, respectively, which are higher than 224 Wh/kg and 4,244 W/kg of VOH as shown in Ragone plot ( FIG. 19 ). Voltage hysteresis collected at 4 A/g exhibit the remarkable differences between the two, but this essential indicator for evaluating the practical possibility is ignored in the current reports on zinc ion batteries. As shown in  FIG. 4D , MnVOH, at the initial cycle(s), delivers a higher specific capacity of 251 mA/g with a mid-value voltage of 0.61 V, which are higher than the specific capacity of 216 mAh/g and 0.47 V in VOH. At the 50 th  cycles, the specific capacity of MnVOH has a slight increase to 275 mAh/g and an increased mid-value voltage of 0.67 V. However, VOH presents a decrease on specific capacity to 92 mAh/g with a slight increased mid-value voltage of 0.51 V. More importantly, energy efficiency (EE), defined by the ratio of discharge and charge energy densities in a battery performance to evaluate the practicability, is 70% calculated in the 50th cycle of MnVOH and its initial EE is 59%. The hysteresis area encompassed by the charging and discharging curves in  FIG. 4E  reflects the energy loss in one cycle. The larger area means lower EE and higher energy loss in the battery. For VOH, it has an initial EE of 40% ( FIG. 20 ) and maintains at 41% in the 50 th  cycle, meaning an energy loss reaches up to ˜60%. Voltage degradations ( FIG. 4F ) on the shelf, another practical parameter to evaluate batteries&#39; self-discharge, were also monitored after the fully charging process at a current density of 50 mA/g. Open circuit voltage of MnVOH battery maintains at 1.36 V (85% of the cutoff voltage) after 50 days, but VOH degrades to 1.29 V, suggesting a less self-discharge reaction happens in MnVOH. Generally, the voltage degradation on the shelf comes from the charge redistribution and reverse ion transport between two electrodes. The better electrochemical performances in MnVOH can be attributed to the introduced Mn (II) that combined with water to expand the interlayer spacing for benefiting the ion diffusion to enhance the rate capability and decrease the polarizations at a high current density. Mn (II) cation carries positive charge that would form chemical interaction with terminal oxygen from [VO n ] layers to stabilize the crystal structure, which guarantees the structural stability under the fast Zn ion insertion and extraction and decrease the ion self-diffusion to restrain the degradation on open circuit voltage when batteries are on the shelf with a long time. In addition, V 4+  induced by Mn (II) is positive effect for the improved electrochemical performance owing its larger ionic radius and one electron in the 3d orbital, which lead to a more expanded lattice spacing and enhanced electrical conductivity to catalyze the phase transition. 
     To confirm the charge storage mechanism, the phase transitions in the electrochemical processes were detected by ex-situ XRD and the patterns are shown in  FIG. 5A . The pristine electrode was fully discharged to 0.2 V, the strongest peak at 6.8° moves to a lower angle of 6.2° meaning the interlayer spacing expanded to 14.1 Å from 12.9 Å. Zn ion has an ionic diameter of 0.88 Å in a six-coordination, but the size of hydrated Zn 2+  with six water molecules is around 2.1 Å, suggesting Zn ions are desolvated before intercalating. In the fully charged state, the peak at the lowest angle goes back to around the starting position, meaning a highly reversible reaction. The peaks around 35° and 62° present the similar tracks. Several weak peaks appear and vanish reversibly in the charging or discharging process, suggesting the reversible phases form in the reactive processes. Most of V cations reduce from 5+ to 4+ and 3+ when MnVOH cathode is discharged to 0.2 V from the pristine as presented in H 2 V 3 O 8 .  FIG. 5B  shows the peak at 517.0 eV corresponding to V 4+  and 515.9 eV to 3+. The characteristic peak about V 5+  can be found owing to the incomplete reaction because the delivered specific capacity of 416 mAh/g at 50 mA/g ( FIG. 4A ) is lower than the theoretical capacity of 598 mAh/g based on the chemical valence of V 5+  fully reduces to V 3+  in the reaction. At the fully charged state, V cations are oxidized to 5+ with a small amount of 4+ as found in the pristine state. It is worth noting that the peak position of V 5+  shifts from 517.4 to 517.6 eV after the full charge ( FIG. 5C ). In general, electron binding energy is defined as the extent of the attraction between cations and electrons through electromagnetic force in a respective atom, ion, molecule or solid, and determined by the electrostatic force of nuclei and screening effect from neighboring electrons, the formation of chemical bonds causes electron redistribution in atoms or ions and further leads to a change on binding energy. The binding energy of V 5+  shifts to a higher energy state, on one hand, can be attributed to the amount of V 4+  from 18.9% to 10.4% calculated by the area ratio in the simulated XPS results. The amount of V 4+  decreases and results in a weaker attraction from the nuclei of V 4+  to the electrons in V 5+  as observed in hydrogenated V 2 O 5 . The amount of V 4+  decrease also explains the capacity increase in the first two cycles as observed in  FIG. 4A . The trapped Zn 2+  ( FIG. 5D ) is another possible reason because it impairs the electron-withdrawing effect of oxygen from the V cation, the reduced ionic diameter in V 5+  in comparison with that of V 4+  means the nucleus has an enhanced interaction on the electrons. The charging specific capacity is higher than the discharging one, which indicates the lower valence V cations are oxidized to 5+ in the first cycle ( FIG. 4A ) as observed in  FIG. 5C . A part of the detected Zn 2+  in the fully charged state may also come from the surface adsorbed or lattice trapped Zn 2+ . Mn (II) was detected by XPS in both fully discharged and charged states ( FIG. 21 ), meaning Mn (II) stays intact in the host crystal. Besides, the oxidation of Mn (II) would occur only at voltages above 1.62 V, thus Mn (II) would not participate redox reactions in the working voltages of MnVOH. EDS mapping in  FIG. 5E  and  FIG. 5F  shows the element signals at fully discharged and charged states, Zn presents a strong and weak signal after discharging and charging in MnVOH cathode, and the reversible stripping/plating reaction simultaneously proceeds on Zn metal anode as observed by SEM ( FIG. 22 ), which means Zn-ion intercalation/deintercalation reversibly happened in the electrochemical processes. The detected Mn in both states implies it stays stable as a pillar in the crystal lattice. The recovered phases and chemical valence of constituent elements in the electrochemical processes demonstrate a reversible intercalation reaction for MnVOH with the redox pairs from the V cations. 
     To discern the reasons of the disparity on the electrochemical performance of both samples, GITT plots were collected at a current density of 50 mA/g as shown in  FIG. 6A . The relaxation rest after charging and discharging causes the zigzag voltage profiles and the voltage recovery is used to evaluate the ion diffusion and the IR drop can be transform to internal reactive resistance (RR). The RRs are calculated using IR drop with the applied current density and the resistances at different steps are show in  FIG. 6B . For MnVOH, the RRs are lower than 0.3 Ω·g in the whole process, even though a resistance bump appears around 1.0 V in the charging process. However, the RRs of VOH present an increase at the charging process and reach the maximum of 0.9 Ω·g around 1.0 V and then go down. In the discharging process, the RRs of MnVOH maintain stable, but two concaves appear at 0.5 and 1.0 V in VOH. It is interesting that the positions of the bumps or concaves are identical to the redox peaks observed in CVs ( FIG. 3B ), implying a radical difference on charge transfer in both samples. From the point of crystal structures, charge transfer in VOH prefers along the ab plane owing to the [VO n ] polyhedra connecting to each other through edge- or point-sharing, but no points or edge contact between the interlayers along the c-axis. In MnVOH, Mn (II) ions reside into and connect [VO] interlayers so that the charge transfer is 3-dimensional and the charges from redox reaction can be transferred easily. EIS spectra ( FIG. 6C ) compare the impedances of batteries before cycle and at the fully charged states and Table 3 lists their charge transfer resistances (CTRs). EIS spectra consist of semi-circle at high-frequency region corresponding to charge transfer resistance and a linear tail at low-frequency relating to ion diffusion. MnVOH presents a CTR of 63Ω at the initial state and the CTR decreases to 24Ω after 3 cycles, while CTRs of VOH are 177 and 38Ω before and after cycling. The decrease of CRTs after cycling might be attributed to the activation of materials and a small amount of trapped Zn 2+  connected the [VO n ] interlayers to provide more charge transfer pathways. The relationship between low-frequencies and real part of impedance ( FIG. 6D ) can be used to calculate the Zn-ion diffusion coefficient. For example, Zn-ion diffusion coefficients of MnVOH and VOH electrodes can be calculated from the low-frequency plots of EIS spectra based on the following equations 
         Z′=R   s   +R   f   +R   ct +σ w ω −0.5 ,  (2)
 
         D   Li+   =R   2   T   2 /2 A   2   n   4   F   4   C   2 σ w   2 ,  (3)
 
     where ω, A, n, F, C, R, and T stands for the angular frequency, electrode area (0.875 cm 2 ), reactive electron number per chemical formula (4), Faraday&#39;s constant (96, 500 C mol −1 ), the molar concentration of Zn ions (3.0×10 −3  mol cm −3 ), gas constant (8.314 J mol −1  K −1 ), and the testing temperature (298 K), respectively. σw is the linear slopes from the relationship between frequencies and real part of impedance ( FIG. 6D ). MnVOH has a higher D Zn2+  of 3.22×10 −12  than that of 1.46×10 −12  cm 2 /s in VOH after the material activation. The lower RRs and CRTs and higher D Zn2+  in MnVOH guarantee the fast redox reaction and stable crystal structure supported by pillar Mn (II) endows the excellent cycling stability at high current density of 4 A/g as shown in  FIG. 4B . 
     
       
         
           
               
             
               
                 TABLE 3 
               
             
            
               
                   
               
               
                 The charge transfer resistances and ion 
               
               
                 diffusion coefficients from the EIS tests 
               
            
           
           
               
               
               
               
               
            
               
                   
                 Samples ID 
                 Label 
                 R ct  (Ω) 
                 D Zn2+ (cm 2 /s) 
               
               
                   
                   
               
               
                   
                 VOH 
                 Before cycling 
                 177 
                 1.20 × 10 −14   
               
               
                   
                   
                 After 3 cycles 
                  38 
                 1.46 × 10 −12   
               
               
                   
                 MnVOH 
                 Before cycling 
                  63 
                 6.07 × 10 −14   
               
               
                   
                   
                 After 3 cycles 
                  24 
                 3.22 × 10 −12   
               
               
                   
                   
               
            
           
         
       
     
     As described herein, Mn (II) expanded VOH achieves the structural stability and reduces reactive polarization during the repeated charge/discharge process. Other transition metal cations such as nickel and cobalt sulfates can also be used as the raw materials to replace manganese sulfate in the synthesis processes to obtain the stabilized samples. The resulting powders exhibit similar XRD patterns as shown in  FIG. 7A , suggesting three samples have the similar crystal structures with MnVOH as characterized and analyzed above. The comparison on rate capability and cycling stability are shown in  FIGS. 7A, 7B, 7C . Ni (II) vanadate (NiVO) and Co (II) vanadate (CoVO) deliver enhanced rate capability and display the excellent cycling stability at 4 A/g and high capacity retentions of 92% and 95%, respectively. Those are higher than 65% of VOH or ˜80 of Zn 0.25 V 2 O 5 .nH 2 O or ˜90% of Na 2 V 6 O 16 .1.63H 2 O in the reported, demonstrating the TMCs introduction can effectively improve the Zn-ion storage performance in hydrated vanadate. The disparities on electrochemical performances of different TMCs vanadate might be attributed to the ionic size of TMCs. Consequently, TMCs introduction in hydrated vanadate is a general and effective strategy to improve the electrochemical performances for various multivalent ions storage. 
     Expanding the interplanar spacing of hydrated vanadate by introduction of Mn (II) ions makes the cathode more thermally and structurally stable. Chemically inserted Mn (II) ions connect [VO n ] layers by chemical bonds, work as pillars making the robust structure, and induce the formation of V 4+  ions resulting in expanded lattice spacing, which facilitates fast ion diffusion (3.22×10 −12  cm 2 /s) and enhances the electrical conductivity. MnVOH cathode possesses a large storage capacity (260 mAh/g) at a higher discharge current density (4 A/g) than that of VOH. MnVOH also demonstrates a capacity retention of 96% over 2,000 cycles at 4 A/g compared to 65% of VOH over 500 cycles. Chemically inserted Mn (II) ions improved reversibility by reducing the voltage polarization, resulting in an energy efficiency of 70% in MnVOH cathode battery, much higher than 40% for VOH at 4 A/g and with an open circuit voltage of MnVOH battery retained at 1.36 V (85% of the cutoff voltage) after 50 days on the shelf. Divalent transition metal cations, such as Co and Ni, exhibit the same structures and stable cycling performance, suggesting that expanded VOH by introduction of TMCs is an effective and universal approach to improve or design high-performance cathode materials for aqueous Zn-ion and other multivalent ions batteries. 
     As discussed above, transition metal stabilized VOH (TMVOs) can be used in a number of settings. For example, TMVOs can be used as electrode materials for aqueous Li- and Al-ion capacitors. The voltage profiles of various TMVOs in Li- and Al-ion capacitors are shown in  FIGS. 8A and 8B , respectively. In aqueous Li-ion capacitors, 1 M LiNO 3  water-based solution was used as the electrolyte and the saturated calomel electrode (SCE) was used as reference electrode and platinum foil was used as the counter electrode. TMVOs can deliver a specific capacity as high as 220 F/g at 1.0 A/g that is higher than 175 F/g of VOH. In aqueous Al-ion capacitors, 1 M Al 2 (SO 4 ) 3  was used as the electrolyte, the counter and reference electrodes are same as used in Li-ion capacitors. The highest specific capacity reaches 540 F/g at 1.0 A/g, it is higher than 140 F/g of VOH. These cathode materials can also be used in nonaqueous Li- and Na-ion batteries. The voltage profiles of the various TMVOs in nonaqueous Li- and Na-ion batteries are shown in  FIGS. 9A and 9B . Li and Na metals were used as anodes in the testing Li- and Na-ion batteries, respectively. 
     Non-transition metal ions, such as Al (III), Mg (II), K (I) and Ca (II), can also be used to create stabilized VOH. Al (III), Mg (II), K (I) and Ca (II) stabilized VOH can be synthesized by the same procedures as in TMVOs synthesis. XRD patterns in  FIG. 10  show the similar results as observed in TMVOs materials, meaning there are likely similar crystal structures in the samples. Moreover, AlVOH delivers a specific capacity of 340 mAh/g at the current density of 500 mA/g ( FIG. 11 ). MgVOH displays a promising application in aqueous Mg-ion batteries in which metallic Mg foil was used as the anode and 4M Mg(TFSI) 2  solution was used as the electrolyte. For example, it can deliver a specific capacity of 260 mAh/g at a current density of 100 mA/g ( FIG. 12 ). 
     Example 2. Preparation and Testing of Additional Cation-Expanded Hydrated Vanadates 
     A series of cation-expanded hydrated vanadates were prepared through similar methods as disclosed in Example 1 regarding MnVOH. The synthesis of the hydrated vanadates simply substituted sulfates having the desired cation instead of manganese sulfate (as used in Example 1). The vanadate hydrates were characterized using similar techniques to those disclosed in Example 1, including XRD and voltage profiling to determine specific capacity. The tested vanadate hydrates and a summary of their synthesis and characterization are presented below in Table 4 and the related summaries and FIGURES below. 
     
       
         
           
               
             
               
                 TABLE 4 
               
             
            
               
                   
               
               
                 Comparison on vanadate hydrates as Zn-ion cathodes. 
               
            
           
           
               
               
               
               
               
            
               
                   
                   
                   
                   
                 Testing 
               
               
                 Cation 
                 Performance 
                 Synthesis 
                 Phases 
                 Conditions 
               
               
                   
               
               
                 Ca 2+   
                 355 mAh/g at 0.5 A/g 
                 Same procedure 
                 Similar XRD 
                 Same 
               
               
                 Mg 2+   
                 410 mAh/g at 0.5 A/g 
                 as used for 
                 patterns to 
                 conditions 
               
               
                 K +   
                 410 mAh/g at 0.5 A/g 
                 MnVOH, in 
                 MnVOH (see 
                 including the 
               
               
                 Al 3+   
                 380 mAh/g at 0.05 A/g 
                 Example 1 
                 FIGS. 23A, 
                 voltage 
               
               
                 Mn 2+   
                 415 mAh/g at 0.05 A/g 
                 just with 
                 24A, and 25A 
                 window and 
               
               
                 Fe 2+   
                 260 mAh/g at 0.5 A/g 
                 different sulfates. 
                 as examples) 
                 battery 
               
               
                 Co 2+   
                 380 mAh/g at 0.5 A/g 
                   
                   
                 assembly as 
               
               
                 Ni 2+   
                 337 mAh/g at 0.5 A/g 
                   
                   
                 MnVOH in 
               
               
                 Cu 2+   
                 379 mAh/g at 0.5 A/g 
                   
                   
                 Example 1. 
               
               
                 Zn 2+   
                 360 mAh/g at 0.5 A/g 
               
               
                   
               
            
           
         
       
     
     CaVOH Cathode Tested in an Aqueous Zn-Ion Battery. 
     Synthesis: the same procedure as used for MnVOH in Example 1, just replace the MnSO4 with CaSO4. 
     Phase:  FIG. 23A  is an XRD pattern of CaVOH. 
     Performance: 355 mAh/g at 0.5 A/g. 
       FIG. 23B  is a voltage profile of CaVOH at 0.5 A/g current density. 
     KVOH Cathode Tested for an Aqueous Zn-Ion Battery. 
     Synthesis: the same procedure as used for MnVOH in Example 1, just replace the MnSO4 with K2SO4. 
     Phase:  FIG. 24A  is an XRD pattern of KVOH. 
     Performance: 410 mAh/g at 0.5 A/g. 
       FIG. 24B  is a voltage profile of KVOH across a range of current densities. 
     AlVOH Cathode Tested for an Aqueous Zn-Ion Battery. 
     Synthesis: the same procedure and similar receipt as used for MnVOH in Example 1, just replace the MnSO4 with Al2(SO4)3. 
     Phase:  FIG. 25A  is an XRD pattern of AlVOH. 
     Performance: 380 mAh/g at 0.05 A/g. 
       FIG. 25B  is a voltage profile of AlVOH at 50 mA/g current density. 
     In these examples tests, the electrode has a mass loading exceeding 4 mg/cm 2  or 1.6 mAh/cm 2 . It can be increased to 12 mg/cm 2  or 4.8 mAh/cm 2  or greater, particularly if needed to meet the current commercial requirements in Li-ion technology. 
     Unless the context clearly requires otherwise, throughout the description and the claims, the words “comprise,” “comprising,” and the like are to be construed in an inclusive sense, as opposed to an exclusive or exhaustive sense; that is to say, in the sense of “including, but not limited to.” As used herein, the terms “connected,” “coupled,” or any variant thereof, means any connection or coupling, either direct or indirect, between two or more elements; the coupling of connection between the elements can be physical, logical, or a combination thereof. Additionally, the words “herein,” “above,” “below,” and words of similar import, when used in this application, shall refer to this application as a whole and not to any particular portions of this application. Where the context permits, words in the above Detailed Description using the singular or plural number may also include the plural or singular number respectively. The word “or,” in reference to a list of two or more items, covers all of the following interpretations of the word: any of the items in the list, all of the items in the list, and any combination of the items in the list. As used herein, the term “about” indicates that the referenced value can be modified plus or minus 5% and still fall within the disclosed embodiment. 
     The above detailed description of embodiments of the present technology is not intended to be exhaustive or to limit the present technology to the precise form disclosed above. While specific embodiments of, and examples for, the present technology are described above for illustrative purposes, various equivalent modifications are possible within the scope of the present technology, as those skilled in the relevant art will recognize. The teachings of the present technology provided herein can be applied to other systems, not necessarily the system described above. The elements and acts of the various embodiments described above can be combined to provide further embodiments. All of the above patents and applications and other references, including any that may be listed in accompanying filing papers, are incorporated herein by reference. Aspects of the present technology can be modified, if necessary, to employ the systems, functions, and concepts of the various references described above to provide yet further embodiments of the present technology. 
     These and other changes can be made to the present technology in light of the above Detailed Description. While the above description details certain embodiments of the present technology and describes the best mode contemplated, no matter how detailed the above appears in text, the present technology can be practiced in many ways. Details of the system may vary considerably in its implementation details, while still being encompassed by the present technology disclosed herein. As noted above, particular terminology used when describing certain features or aspects of the present technology should not be taken to imply that the terminology is being redefined herein to be restricted to any specific characteristics, features, or aspects of the present technology with which that terminology is associated. In general, the terms used in the following claims should not be construed to limit the present technology to the specific embodiments disclosed in the specification, unless the above Detailed Description section explicitly defines such terms. Accordingly, the actual scope of the present technology encompasses not only the disclosed embodiments, but also all equivalent ways of practicing or implementing the present technology. 
     While illustrative embodiments have been illustrated and described, it will be appreciated that various changes can be made therein without departing from the spirit and scope of the invention.